### Delft University of Technology

### Mechanical properties of additively manufactured thick honeycombs

Hedayati, Reza; Sadighi, Mojtaba; Mohammadi-Aghdam, M; Zadpoor, Amir DOI

10.3390/ma9080613 Publication date 2016

Document Version Final published version Published in

Materials

Citation (APA)

Hedayati, R., Sadighi, M., Mohammadi-Aghdam, M., & Zadpoor, A. (2016). Mechanical properties of additively manufactured thick honeycombs. Materials, 9(8), 1-23. [613]. https://doi.org/10.3390/ma9080613

Important note

To cite this publication, please use the final published version (if applicable). Please check the document version above.

Copyright

Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy

Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.

This work is downloaded from Delft University of Technology.

**materials**

**materials**

Article

**Mechanical Properties of Additively Manufactured**

**Thick Honeycombs**

**Reza Hedayati1,2,*, Mojtaba Sadighi1, Mohammad Mohammadi Aghdam1**

**and Amir Abbas Zadpoor2**

1 _{Department of Mechanical Engineering, Amirkabir University of Technology (Tehran Polytechnic),}

Hafez Ave, Tehran 158754413, Iran; [email protected] (M.S.); [email protected] (M.M.A.)

2 _{Department of Biomechanical Engineering, Faculty of Mechanical, Maritime, and Materials Engineering,}

Delft University of Technology (TU Delft), Mekelweg 2, Delft 2628 CD, The Netherlands; [email protected]

***** Correspondence: [email protected] or [email protected] or [email protected];

Tel.: +31-15-2781021

Academic Editor: Juergen Stampfl

Received: 8 May 2016; Accepted: 8 July 2016; Published: 23 July 2016

**Abstract:**Honeycombs resemble the structure of a number of natural and biological materials such
as cancellous bone, wood, and cork. Thick honeycomb could be also used for energy absorption
applications. Moreover, studying the mechanical behavior of honeycombs under in-plane loading
could help understanding the mechanical behavior of more complex 3D tessellated structures such as
porous biomaterials. In this paper, we study the mechanical behavior of thick honeycombs made
using additive manufacturing techniques that allow for fabrication of honeycombs with arbitrary and
precisely controlled thickness. Thick honeycombs with different wall thicknesses were produced from
polylactic acid (PLA) using fused deposition modelling, i.e., an additive manufacturing technique.
The samples were mechanically tested in-plane under compression to determine their mechanical
properties. We also obtained exact analytical solutions for the stiffness matrix of thick hexagonal
honeycombs using both Euler-Bernoulli and Timoshenko beam theories. The stiffness matrix was then
used to derive analytical relationships that describe the elastic modulus, yield stress, and Poisson’s
ratio of thick honeycombs. Finite element models were also built for computational analysis of the
mechanical behavior of thick honeycombs under compression. The mechanical properties obtained
using our analytical relationships were compared with experimental observations and computational
results as well as with analytical solutions available in the literature. It was found that the analytical
solutions presented here are in good agreement with experimental and computational results even
for very thick honeycombs, whereas the analytical solutions available in the literature show a large
deviation from experimental observation, computational results, and our analytical solutions.
**Keywords:**cellular structures; 3D printing; elastic properties; hexagonal honeycomb

**1. Introduction**

Bone has the intrinsic ability of self-healing in the case of being damaged in small areas. However, in large bony defects, bone loses its ability to repair itself by regeneration of new bony tissue. While autologous bone grafting is known as the gold standard in orthopaedic surgery, it has some drawbacks such as limited bone stack and donor site mordibility [1]. Recently, porous titanium and titanium alloy scaffolds have been thoroughly investigated due to their excellent biocompatibility and corrosion resistance, low stiffness (which is necessary for avoiding stress shielding), and good bone regeneration performance.

Additive manufacturing techniques have made it possible to fabricate scaffolds with precisely controlled micro-architecture. Therefore, several 3D unit cell types have been suggested and tested

**Materials 2016, 9, 613** 2 of 23

mechanically and biologically when used as the micro-architecture of bone replacing scaffolds [2,3]. Singh showed that in some areas (where bone is very dense), cancellous bone microarchitecture resembles that of a hexagonal honeycomb with thick cell walls [4]. Hexagonal honeycombs or honeycomb-like structures have been manufactured as biomedical implants using different additive manufacturing techniques [5,6]. Recently, various cells have been successfully cultured in collagen scaffold honeycombs [7–9]. It is important to study the mechanical behavior of thick honeycomb-like structures, because the mechanical properties of the biomaterials used for tissue regeneration could significantly influence the tissue regeneration performance of biomaterials.

The mechanical properties of honeycombs (such as their stiffness and yield stress) in out-of-plane direction are usually much higher compared to their in-plane properties. This is why more studies have been devoted to the investigation of out-of-plane properties of honeycombs compared to their in-plane properties. However, honeycombs are loaded in-plane in a number of natural structures such as cancellous bone, wood, and cork [10]. Moreover, thick honeycombs could be also useful for energy absorption purposes in the in-plane direction. In this case, the mechanism dominating the structure deformation is bending of the cell walls (rather than sudden buckling of the walls which is common in the out-of-plane deformations of honeycombs) and then face-to face crushing of the cell walls. This can lead to a smoother stress-strain curve with higher energy absorption capacity as compared to the out-of-plane direction, if the geometrical parameters are chosen properly.

Several experimental works have been carried out on the in-plane deformation of honeycombs. Foo et al. [11] obtained linear elastic mechanical properties of Nomex™ honeycomb structures using extensive test programs and compared their results with those of their finite element (FE) models. They observed size effects for the moduli of Nomex™ honeycombs. Papka and Kyriakides [12] compressed honeycomb specimens between stiff flat grips experimentally and numerically. They found out that although the crushing patterns developed during the plateau regime differs from specimen to specimen (caused by specimen size and geometric imperfections), the cell failure mechanism is similar for all cases. Other experimental works on the in-plane mechanical behavior of honeycombs can be found in [13–17]. Several numerical studies have also been carried out using FE methods the most important of which are in the following references [18–20].

El-Sayed et al. [21] published the first analytical study on the in-plane mechanical properties
of hexagonal honeycombs in which the elastic mechanical properties of a composite under in-plane
axial and out-of-plane bending loads were studied, and the plastic deformation properties under
in-plane axial loading were characterized. However, as stated in [10], their work had ‘numerous small
errors’ which rendered the results unreliable. In 1982, Gibson et al. [10] presented improved analytical
relationships for the mechanical properties of hexagonal honeycombs (E1, E2*, υ*12*, υ*21*, σ*y1*, σ*y2, G, and
*σ*el). Their results showed good agreement with their experimental results for both rubber and metal
honeycombs but only for very small values of wall thickness and relative density.

Masters and Evans [22] developed an analytical model for prediction of elastic constants of
honeycombs by decomposing the general deformation of a honeycomb cell into flexural, stretching,
and hinging parts. For each of the three mechanisms, force constants were defined while relationships
for E1, E2*, υ*12*, υ*21, and G were calculated. The elastic constants calculated from each mechanism were
then superimposed to give a general model [23]. Masters and Evans [22] did not obtain any relationship
for yield stress. Goswami [24] derived analytical formulas for the elastic properties of hexagonal
honeycomb cores. Elemental beam theory was used for each component inside the unit cell to give
different elastic properties by means of strain energy concept. The results of their model coincided
with the results reported in [10]. Balawi and Abot [25] presented a modified model for commercial
hexagonal honeycombs having double wall thickness in vertical walls and some curvature in the
neighborhood of cell vertices caused by expansion or corrugation processes during manufacturing.

In all of the above-mentioned works, the Euler-Bernoulli beam theory is the theoretical basis for deriving the analytical relationships. The analytical solutions obtained using the Euler-Bernoulli beam theory are not applicable to thick honeycombs, because a number of simplifying assumptions are used

**Materials 2016, 9, 613** 3 of 23

in that theory. It is therefore important to use the Timoshenko beam theory for deriving the analytical relationships that are used for thicker honeycombs (which can be good candidates for replacing dense cancellous bones). In this paper, the stiffness matrix of hexagonal honeycomb structures is obtained by which the elastic properties of honeycomb structures including the elastic modulus, Poisson’s ratio, and yield stress in both major in-plane directions are found. The results obtained from the derived formulas are compared with existing analytical formulas presented by Gibson and Ashby [10] and Masters and Evans [22] as well as to the experimental results of the study of Gibson and Ashby [10] on low density honeycombs, and with the mechanical properties measured for additively manufactured dense honeycombs in this study. Moreover, FE models are created to validate the proposed analytical relationships and to present the steps required for development of a trustworthy numerical tool for investigation of thick honeycomb structures.

**2. Materials and Methods**
2.1. Experimental Tests

An additive manufacturing technique, i.e., fused deposition modelling, was used for fabricating thick honeycombs with a wide range of relative densities from polylactic acid (PLA). The hexagonal honeycombs were made from poly-lactic acid (PLA) filaments using 5th generation Replicator Desktop Makerbot 3D printer. For each density, six samples were made (three sample for testing in each of the two main directions of each honeycomb). The dimensions of the hexagonal honeycombs were 77 ˆ 90 ˆ 21.395 cm3. Four different relative densities of honeycombs were generated by varying the thickness to length ratio of the cell walls, i.e., t{l “ 0.09, t{l “ 0.18, t{l “ 0.27, and t{l “ 0.36 (Figure 1). The mechanical properties of the samples were measured under compression using INSTRON 5985 machine (Illinois Tool Works Inc., Glenview, IL, USA) with 100 kN load cells. The displacement rate of the upper grip was set to 2 mm/min. The tests and elastic properties calculations were in accordance with the specifications described in the standard ISO 13314:2011 [26]. To measure the mechanical properties of the bulk material, i.e., additively manufactured PLA used in the current study, bulk cylinders (100% infill) with nominal diameters of 12.7 mm and nominal lengths of 25.4 mm were made and tested under compression using a methodology similar to that of the honeycombs. The measured elastic modulus and yield stress of the bulk material were 1.962 ˘ 0.069 GPa and 56.204 ˘ 1.213 MPa, respectively. To gain a better overview of the elastic modulus and yield stress values, their normalized values (i.e., ratio of their value in the porous structure to their corresponding value in the bulk material) were plotted and compared between the analytical, numerical, and experimental values.

* Materials 2016, 9, 613 * 3 of 23

In all of the above-mentioned works, the Euler-Bernoulli beam theory is the theoretical basis for
deriving the analytical relationships. The analytical solutions obtained using the Euler-Bernoulli
beam theory are not applicable to thick honeycombs, because a number of simplifying assumptions
are used in that theory. It is therefore important to use the Timoshenko beam theory for deriving the
analytical relationships that are used for thicker honeycombs (which can be good candidates for
replacing dense cancellous bones). In this paper, the stiffness matrix of hexagonal honeycomb
structures is obtained by which the elastic properties of honeycomb structures including the elastic
modulus, Poisson’s ratio, and yield stress in both major in-plane directions are found. The results
obtained from the derived formulas are compared with existing analytical formulas presented by
Gibson and Ashby [10] and Masters and Evans [22] as well as to the experimental results of the study
of Gibson and Ashby [10] on low density honeycombs, and with the mechanical properties
measured for additively manufactured dense honeycombs in this study. Moreover, FE models are
created to validate the proposed analytical relationships and to present the steps required for
development of a trustworthy numerical tool for investigation of thick honeycomb structures.
**2. Materials and Methods **

*2.1. Experimental Tests *

An additive manufacturing technique, i.e., fused deposition modelling, was used for fabricating thick honeycombs with a wide range of relative densities from polylactic acid (PLA). The hexagonal honeycombs were made from poly-lactic acid (PLA) filaments using 5th generation Replicator Desktop Makerbot 3D printer. For each density, six samples were made (three sample for testing in each of the two main directions of each honeycomb). The dimensions of the hexagonal honeycombs were 77 × 90 × 21.395 cm . Four different relative densities of honeycombs were generated by varying the thickness to length ratio of the cell walls, i.e., / = 0.09, / = 0.18, / = 0.27, and / = 0.36 (Figure 1). The mechanical properties of the samples were measured under compression using INSTRON 5985 machine (Illinois Tool Works Inc., Glenview, IL, USA) with 100 kN load cells. The displacement rate of the upper grip was set to 2 mm/min. The tests and elastic properties calculations were in accordance with the specifications described in the standard ISO 13314:2011 [26]. To measure the mechanical properties of the bulk material, i.e., additively manufactured PLA used in the current study, bulk cylinders (100% infill) with nominal diameters of 12.7 mm and nominal lengths of 25.4 mm were made and tested under compression using a methodology similar to that of the honeycombs. The measured elastic modulus and yield stress of the bulk material were 1.962 ± 0.069 GPa and 56.204 ± 1.213 MPa, respectively. To gain a better overview of the elastic modulus and yield stress values, their normalized values (i.e., ratio of their value in the porous structure to their corresponding value in the bulk material) were plotted and compared between the analytical, numerical, and experimental values.

**(a) (b)**

**Materials 2016, 9, 613** 4 of 23

* Materials 2016, 9, 613 * 4 of 23

**(c) (d)**

**Figure 1. The manufactured hexagonal honeycombs with (a) t/l = 0.09; (b) t/l = 0.18; (c) t/l = 0.27; and **

**(d) t/l = 0.36. **

*2.2. Relative Density *

A unit cell (Figure 2b) constructing a 2D hexagonal lattice structure (Figure 2a) consists of four vertical and four inclined edges. The lengths of the vertical and inclined edges are assumed to be possibly different and are denoted by and ℎ, respectively. The angle between the inclined edges and the axis is also arbitrary and is denoted by . The thickness of the edges is however considered constant throughout the study. It is customary in the studies investigating cellular solids to express the mechanical properties as functions of relative density (also called apparent density) rather than other geometrical parameters such as / . Dealing with relative density ( ) rather than other geometrical parameters gives a better overview of the weight of the structure, and also makes it easier to compare the mechanical properties of structures with different micro-geometrical features but of the same weight.

In thin honeycombs, i.e., when the ratio / is very small, the area occupied by the material constructing half a unit cell (Figure 3) is 2( + + ). On the other hand, the total area occupied by half a unit cell is (2ℎ + 2 ) from which the relative density is given by

= =_{2(ℎ +}(ℎ + 2 )_{)} (1)

In thick honeycombs, the area occupied by the material of half a unit cell is (see Figure 3)
= 2 1_{2} ℎ_{2}−_{2 sin} +_{2}ℎ+_{2}cot −_{2 sin} _{2}+_{sin} sin

+1

2 2 ℎ −sin + ℎ −sin + cot = ℎ −sin +2cot + 2

(2)

from which the relative density can be calculated as

= = ℎ + 2 − sin + 2cot_{2(ℎ +} _{)} (3)

Plotting the simplified and exact relative density relationships (i.e., Equations (1) and (3)) for regular hexagonal honeycombs showed that their values are close regardless of / (see Figure 4). Therefore, Equation (1) will be used from now on for calculating relative density because of its simplicity and also due to its use in the work by Gibson and Ashby [10,27].

**Figure 1.** **The manufactured hexagonal honeycombs with (a) t/l = 0.09; (b) t/l = 0.18; (c) t/l = 0.27;**

**and (d) t/l = 0.36.**

2.2. Relative Density

A unit cell (Figure2b) constructing a 2D hexagonal lattice structure (Figure 2a) consists of
four vertical and four inclined edges. The lengths of the vertical and inclined edges are assumed
to be possibly different and are denoted by l and h, respectively. The angle between the inclined
edges and the X2*axis is also arbitrary and is denoted by θ. The thickness of the edges t is however*
considered constant throughout the study. It is customary in the studies investigating cellular solids to
express the mechanical properties as functions of relative density (also called apparent density) rather
than other geometrical parameters such as t{l. Dealing with relative density (* _{ρs}ρ*) rather than other
geometrical parameters gives a better overview of the weight of the structure, and also makes it easier
to compare the mechanical properties of structures with different micro-geometrical features but of the
same weight.

In thin honeycombs, i.e., when the ratio t{l is very small, the area occupied by the material constructing half a unit cell (Figure3) is 2

´ h 2 t 2`lt ` h 2 t 2 ¯

. On the other hand, the total area occupied
*by half a unit cell is p2h ` 2lcos θq l sinθ from which the relative density is given by*

*µ “* *ρ*

*ρ*s

“ t ph ` 2lq

*2 ph ` lcos θq l sinθ* (1)

In thick honeycombs, the area occupied by the material of half a unit cell is (see Figure3)
A “ 2”1_{2}´h_{2}´* _{2sinθ}*t `h

_{2}`

_{2}t

*cotθ ´*t

_{2sinθ}¯ t

2`*sinθ*t *lsinθ*
ı

`1_{2}_{2}t`h ´* _{sinθ}*t `h ´

*t `*

_{sinθ}*tcotθ*˘

“th ´* _{sinθ}*t2 `t

_{2}2

*cotθ ` 2 tl*(2) from which the relative density can be calculated as

*µ “* *ρ*
*ρ*s
“t`h ` 2l ´
t
*sinθ*`2t*cotθ*
˘
*2 ph ` lcos θq l sinθ* (3)

Plotting the simplified and exact relative density relationships (i.e., Equations (1) and (3)) for regular hexagonal honeycombs showed that their values are close regardless of t{l (see Figure4). Therefore, Equation (1) will be used from now on for calculating relative density because of its simplicity and also due to its use in the work by Gibson and Ashby [10,27].

**Materials 2016, 9, 613** 5 of 23

* Materials 2016, 9, 613 * 5 of 23

**(a)**

**(b)**

**(c)**

**Figure 2. (a) A honeycomb structure; (b) a single unit cell of the honeycomb considered for analytical **
**solution; and (c) degrees of freedom acting on the considered unit cell. **

**Figure 2.(a) A honeycomb structure; (b) a single unit cell of the honeycomb considered for analytical**

**Materials 2016, 9, 613** 6 of 23

* Materials 2016, 9, 613 * 6 of 23

**Figure 3. Dimensions of half a unit cell. **

**Figure 4. Comparison of relative density values based on simplified or exact formulas for regular **

hexagonal honeycombs.
*2.3. Euler-Bernoulli Beam Theory *

In this section, we use the Euler-Bernoulli beam theory to derive analytical relationships for the elastic modulus, , Poisson’s ratio, , and yield stress, of hexagonal honeycombs as functions of the elastic modulus, Poisson’s ratio, and yield stress of the bulk material ( , , ) and the relative density ( ) of the honeycomb structure. Since the in-plane deformation of the honeycombs is plane-strain, the problem is solved using beam elements with square cross-section.

The geometry and deformation of a honeycomb unit cell under simple axial loading is

symmetrical with respect to both and directions. Therefore, the deformation of ¼ of a unit

cell is representative of the deformation of all the four quarters. The symmetry of the unit cell with

respect to and also implies that edges AB and A`B` (Figure 2c) remain straight during the

elastic deformation and that they are only contracted or expanded with no additional flexure.

Therefore, each of points A and B have only one degree of freedom denoted by and ,

respectively. Since the deformation of edge CC` in a unit cell is symmetrical with respect to the deformation of edge C``C``` in the neighbouring unit cell located on its left side, similar to edge AB, edge CC` cannot have any rotation or lateral deflection along its length. Therefore, point C can have only two degrees of freedom, which are displacements in the and directions and are denoted and , respectively. Edge BC cannot have any rotation at its ends B and C, but it can bend in its middle part.

As for the bending moment, the Euler–Bernoulli beam equation can be written as

0 0.1 0.2 0.3 0.4 0.5
0
0.1
0.2
0.3
0.4
0.5
**t/l**
**Relative density**
**Simplified formula**
**Exact formula**

**Figure 3.**Dimensions of half a unit cell.

* Materials 2016, 9, 613 * 6 of 23

**Figure 3. Dimensions of half a unit cell. **

**Figure 4. Comparison of relative density values based on simplified or exact formulas for regular **

hexagonal honeycombs.
*2.3. Euler-Bernoulli Beam Theory *

In this section, we use the Euler-Bernoulli beam theory to derive analytical relationships for the elastic modulus, , Poisson’s ratio, , and yield stress, of hexagonal honeycombs as functions of the elastic modulus, Poisson’s ratio, and yield stress of the bulk material ( , , ) and the relative density ( ) of the honeycomb structure. Since the in-plane deformation of the honeycombs is plane-strain, the problem is solved using beam elements with square cross-section.

The geometry and deformation of a honeycomb unit cell under simple axial loading is

symmetrical with respect to both and directions. Therefore, the deformation of ¼ of a unit

cell is representative of the deformation of all the four quarters. The symmetry of the unit cell with

respect to and also implies that edges AB and A`B` (Figure 2c) remain straight during the

elastic deformation and that they are only contracted or expanded with no additional flexure.

Therefore, each of points A and B have only one degree of freedom denoted by and ,

respectively. Since the deformation of edge CC` in a unit cell is symmetrical with respect to the deformation of edge C``C``` in the neighbouring unit cell located on its left side, similar to edge AB, edge CC` cannot have any rotation or lateral deflection along its length. Therefore, point C can have only two degrees of freedom, which are displacements in the and directions and are denoted and , respectively. Edge BC cannot have any rotation at its ends B and C, but it can bend in its middle part.

As for the bending moment, the Euler–Bernoulli beam equation can be written as

0 0.1 0.2 0.3 0.4 0.5
0
0.1
0.2
0.3
0.4
0.5
**t/l**
**Relative density**
**Simplified formula**
**Exact formula**

**Figure 4.** Comparison of relative density values based on simplified or exact formulas for regular

hexagonal honeycombs.

2.3. Euler-Bernoulli Beam Theory

In this section, we use the Euler-Bernoulli beam theory to derive analytical relationships for
*the elastic modulus, E, Poisson’s ratio, ν, and yield stress, σ*yof hexagonal honeycombs as functions
of the elastic modulus, Poisson’s ratio, and yield stress of the bulk material (Es*, σ*ys*, ν*s) and the
*relative density (µ) of the honeycomb structure. Since the in-plane deformation of the honeycombs is*
plane-strain, the problem is solved using beam elements with square cross-section.

The geometry and deformation of a honeycomb unit cell under simple axial loading is symmetrical with respect to both X1and X2directions. Therefore, the deformation of 14of a unit cell is representative of the deformation of all the four quarters. The symmetry of the unit cell with respect to X1and X2 also implies that edges AB and A8B8(Figure2c) remain straight during the elastic deformation and that they are only contracted or expanded with no additional flexure. Therefore, each of points A and B have only one degree of freedom denoted by q1and q2, respectively. Since the deformation of edge CC8 in a unit cell is symmetrical with respect to the deformation of edge C88C888in the neighbouring unit cell located on its left side, similar to edge AB, edge CC8cannot have any rotation or lateral deflection along its length. Therefore, point C can have only two degrees of freedom, which are displacements in the X1and X2directions and are denoted q4and q3, respectively. Edge BC cannot have any rotation at its ends B and C, but it can bend in its middle part.

As for the bending moment, the Euler–Bernoulli beam equation can be written as d4w

**Materials 2016, 9, 613** 7 of 23

where w is the deflection of the mid-surface and x is the coordinate of the considered point. The solution to this differential equation can be expressed as:

w “ c0`c1x ` c2x2`c3x3 (5)

where constants c0´c3must be determined by applying certain boundary conditions. For a cantilever Euler-Bernoulli beam at the free end of which a point load F acts, we have

*δ “* Fl
3

3EsI *and θ “*
Fl2

2EsI (6)

and for a cantilever beam with a concentrated moment M at its end, the displacement and rotation are

*δ “* Ml

2

2EsI *and θ “*
Fl

EsI (7)

In beams that the angle of the free end does not change during the deformation (e.g., the edges of the honeycomb considered in this study), the rotations produced by the lateral load F and moment M must be equal and opposite from which the value of M can be identified:

Fl2 2EsI “ Ml EsI ñ M “ Fl 2 (8)

While the force F tends to increase the lateral displacement, the moment M tends to reduce the deflection (Figure5a). The total deflection resulted from force F and moment M is then

*δ “* Fl
3
3EsI
´ˆ Fl
2
˙
l2
2EsI
“ Fl
3
12EsI (9)

Rewriting Equation (9) as a function of F gives (see Figure5a) F “ 12EsI

l3 *δ* (10)

Similarly, the axial force required to displace the end of a rod by u is AEsu{l (see Figure5). Figure5 will be referred to several times in the rest of the paper for determining the forces and moments.

* Materials 2016, 9, 613 * 7 of 23

= 0 (4)

where is the deflection of the mid-surface and is the coordinate of the considered point. The solution to this differential equation can be expressed as:

= + + + (5)

where constants − must be determined by applying certain boundary conditions. For a cantilever Euler-Bernoulli beam at the free end of which a point load acts, we have

=

3 =2 (6)

and for a cantilever beam with a concentrated moment at its end, the displacement and rotation are

=

2 = (7)

In beams that the angle of the free end does not change during the deformation (e.g., the edges of the honeycomb considered in this study), the rotations produced by the lateral load and moment must be equal and opposite from which the value of can be identified:

2 = ⇒ = 2 (8)

While the force tends to increase the lateral displacement, the moment tends to reduce the deflection (Figure 5a). The total deflection resulted from force and moment is then

=

3 − 2 2 =12 (9)

Rewriting Equation (9) as a function of gives (see Figure 5a)

=12 (10)

Similarly, the axial force required to displace the end of a rod by is / (see Figure 5). Figure 5 will be referred to several times in the rest of the paper for determining the forces and moments.

**Figure 5. Forces and moments required to cause (a) lateral displacement with no rotation at the **
**free end of a beam; and (b) simple axial expansion . **

**Figure 5.****Forces and moments required to cause (a) lateral displacement δ with no rotation at the free**

**Materials 2016, 9, 613** 8 of 23

2.4. Timoshenko Beam Theory

The Timoshenko beam theory takes into account shear deformation and rotational inertia effects, making it suitable for describing the behavior of thick beams. For a homogenous beam of constant cross-section, the governing equations of the Timoshenko beam theory are:

d2
dx2
ˆ
EsI*dϕ*
dx
˙
“q px, tq
dw
dx *“ ϕ ´*
1
*κ AG*s
d
dx
ˆ
EsI*dϕ*
dx
˙ (11)

*where ϕ is the angle of rotation of the normal to the mid-surface of the beam and κ is the shear*
*coefficient factor. The shear coefficient factor is 10 p1 ` ν*sq { p12 ` 11νsqfor a rectangular cross-section
(such as the beams considered in this study). In a linear elastic Timoshenko beam, the bending moment

*M is related to the angle of rotation ϕ by*

M “ ´EsI*B ϕ*

Bx (12)

For a cantilever Timoshenko beam with a point load F at its free end, M “ Fl and Equations (11)
lead to
*δ “* Fl
3
3EsI
` Fl
*κ AG*s *and θ “*
Fl2
2EsI
` F
*κ AG*s (13)

The displacement and rotation of a cantilever Timoshenko beam with a concentrated moment M at its free end are identical to those of a similar Euler-Bernoulli beam. As before, the rotations produced by the lateral load F and moment M must be equal and opposite from which M can be calculated

Fl2
2EsI
` F
*κ AG*s
“ F
?
2
16l2
2EsI
“ Ml
EsI
ñ M “ Fˆ l
2`
EsI
*κ AG*sl
˙
(14)
While F tends to increase the lateral displacement, M tends to reduce it. The total deflection
caused by F and M is then

*δ “* Fl
3
3EsI
` Fl
*κ AG*s
´ˆ Fl
2 `
FEsI
*κ AG*sl
˙
l2
2EsI
“ Fl
3
12EsI
` Fl
*2κ AG*s (15)

Rewriting Equation (15) as a function of F gives

F “ 1
l3
12EsI`
l
*2κ AG*s
*δ* (16)

2.5. Stiffness Matrix Derivation

Due to the symmetry of the hexagonal unit cell,1_{4}of the unit cell was considered for the analytical
study (the top left part of Figure2c). Therefore, the obtained force at points A and B must be multiplied
by two to calculate the total force applied to the corresponding degrees of freedom (DOFs) q1and q2,
respectively. Similarly, the obtained forces for point C must be multiplied by four to give the total force
applied to the third and fourth DOFs, i.e., q3and q4.

In this study, the stiffness matrix of the unit cell is obtained which is then used to calculate the displacements of the DOFs of the structure as functions of the imposed force. Given the displacements of the DOFs, analytical relationships for the mechanical properties of the unit cell can be derived. The displacements of a hexagonal unit cell can be considered as superposition of four distinct displacements taking place at each DOF separately. To obtain the elements of the ith column of the stiffness matrix, DOF qiis displaced by unity while the other DOFs are kept fixed. The forces that

**Materials 2016, 9, 613** 9 of 23

must be applied at each DOF to cause such a deformation constitute column i of the stiffness matrix. By applying this technique to all the DOFs, the elements of all the columns of the stiffness matrix are obtained. The force-displacement relationship of this system has the following form:

$ ’ ’ ’ & ’ ’ ’ % Q1 Q2 Q3 Q4 , / / / . / / / -“ » — — — – k11 k12 k13 k14 k21 k22 k23 k24 k31 k32 k33 k34 k41 k42 k43 k44 fi ffi ffi ffi fl $ ’ ’ ’ & ’ ’ ’ % q1 q2 q3 q4 , / / / . / / / -(17)

where Qiis the external force applied to a DOF qi. In the following, the procedure of obtaining the stiffness matrix elements, kij, is presented. When applying the displacements, it is necessary to know what external forces must be applied at each DOF. Figure5demonstrates the loads required to cause lateral and axial unit displacements at the free end of a cantilever Euler-Bernoulli beam. This figure is referred to several times in the following.

2.5.1. The First DOF: q1“1

In this subsection, the elements of the first column of the stiffness matrix are derived by applying the displacement q1“1 and setting q2“q3“q4“0. This deformation displaces the top and bottom points A and A‘ by unity upwards and downwards, respectively. Due to this deformation, strut AB is axially stretched by unity and applies the force 2AEs

h (see Figure6a) to points A and B. In order to have such a deformation, the forces Q1

2 “ 2AEs h and Q2 2 “ ´ 2AEs

h must be applied to points A and B which give Q1“k11 “4AEhs and Q2“k21“ ´4AEhs. The negative value of Q2implies that in order to keep point B fixed, the external load in point B must be in the opposite direction of q2. Since beams BC and CC8are not affected by this deformation mode, no external force is needed to be applied to point C, hence Q3“k31“Q4“k41 “0.

* Materials 2016, 9, 613 * 9 of 23

stiffness matrix are obtained. The force-displacement relationship of this system has the following form:

= (17)

where is the external force applied to a DOF . In the following, the procedure of obtaining the stiffness matrix elements, , is presented. When applying the displacements, it is necessary to know what external forces must be applied at each DOF. Figure 5 demonstrates the loads required to cause lateral and axial unit displacements at the free end of a cantilever Euler-Bernoulli beam. This figure is referred to several times in the following.

2.5.1. The First DOF: = 1

In this subsection, the elements of the first column of the stiffness matrix are derived by applying the displacement = 1 and setting = = = 0. This deformation displaces the top and bottom points A and A` by unity upwards and downwards, respectively. Due to this deformation, strut AB is axially stretched by unity and applies the force (see Figure 6a) to points A and B. In order to have such a deformation, the forces = and = − must be applied to points A and B which give = = and = = − . The negative value of

implies that in order to keep point B fixed, the external load in point B must be in the opposite direction of . Since beams BC and CC` are not affected by this deformation mode, no external force is needed to be applied to point C, hence = = = = 0.

**Figure 6. Free-body diagrams of struts (a) AB in deformation ** **= 1; (b) AB in deformation ** = 1;

**and (c) BC in deformation ** = 1 of the hexagonal honeycomb unit cell.

2.5.2. The Second DOF: = 1

In this case, beams AB and A`B` go under pure compression. In contrast to case = 1, here we have = − and = (Figure 6b). Unlike the previous case (q = 1), here beam BC does deform (Figure 6c). The displacement of point B can be decomposed into two displacement of perpendicular to the undeformed beam BC and cos along it (Figure 6c). To have such axial and lateral displacements, the forces cos and sin must have been applied to the ends of beam BC (Figure 6c). Equilibrium of forces in the direction at point B gives (Figure 6b,c)

, = 0 → − 2 cos +12 sin −2_{ℎ} + _{2} = 0 (18)

**Figure 6.Free-body diagrams of struts (a) AB in deformation q**1“**1; (b) AB in deformation q**2 “1;

**and (c) BC in deformation q**2“1 of the hexagonal honeycomb unit cell.
2.5.2. The Second DOF: q2“1

In this case, beams AB and A8B8go under pure compression. In contrast to case q1 “ 1, here we have Q1

2 “ ´2AEhs and Q2

2 “ 2AEhs (Figure6b). Unlike the previous case (q1 “1), here beam BC
does deform (Figure6c). The displacement of point B can be decomposed into two displacement of
*sinθ perpendicular to the undeformed beam BC and cosθ along it (Figure*6c). To have such axial and
lateral displacements, the forcesAEs

l *cosθ and*
12EsI

l3 *sinθ must have been applied to the ends of beam*
BC (Figure6c). Equilibrium of forces in the X1direction at point B gives (Figure6b,c)

**Materials 2016, 9, 613** 10 of 23
ÿ
fX1, B“0 Ñ ´2ˆ AEs
l cos
2
*θ `*12EsI
l3 sin
2
*θ*
˙
´2AEs
h `
Q2
2 “0
Ñ Q2“k22“4
ˆ AEs
l cos
2
*θ `*12EsI
l3 sin
2
*θ*
˙
`4AEs
h
(18)

Beam CC8_{is fixed and therefore imposes no forces to point C. Force equilibrium at point C in the}
X1and X2directions gives (Figure6c)

ÿ
fX1, C“0 Ñ ´
ˆ AEs
l *cosθsinθ `*
12EsI
l3 *cosθsinθ*
˙
`Q4
4 “0
Ñ Q4“k42“*4cosθsinθ*
ˆ AEs
l ´
48EsI
l3
˙ (19)
ÿ
fX2, C“0 Ñ AEs
l cos
2
*θ `*12EsI
l3 sin
2
*θ `*Q3
2 “0
Ñ Q3“k32“ ´4
AEs
l cos
2* _{θ ´}*48EsI
l3 sin
2

*(20)*

_{θ}2.5.3. The Third DOF: q3“1

This deformation type displaces vertex C upward by unity. Beam AB does not deform and, thus, does not impose any load to point B. Point A is not influenced by this deformation mode, thus Q1“k13“0. Force equilibrium at point B in the X2direction gives (Figure7a)

ÿ
fX2, B“0 Ñ 2
ˆ AEs
l cos
2
*θ `*12EsI
l3 sin
2
*θ*
˙
`Q2
2 “0
Ñ Q2“k23“ ´4
ˆ AEs
l cos
2* _{θ `}*12EsI
l3 sin
2

*˙ (21)*

_{θ}Beam CC8(with length h and cross-section area of A{2) is stretched by 2 and therefore imposes the force AEs{h to point C. Force equilibrium at point C in the X2direction gives (Figure7a)

ÿ
fX2, C“0 Ñ ´
AEs
l cos
2* _{θ ´}*12EsI
l3 sin
2

*AEs h ` Q3 4 “0 Ñ Q3“k33“ 4AEs l cos 2*

_{θ ´}*48EsI l3 sin2*

_{θ `}*θ `*4AEs h (22)

Similarly, force equilibrium at the same point in the X1direction gives (Figure7a)
ÿ
fX1, C“*0 Ñ cosθsinθ*
ˆ
´AEs
l `
12EsI
l3
˙
`Q4
4 “0
Ñ Q4“k43“*cosθsinθ*
ˆ 48EsI
l3 ´
4AEs
l
˙ (23)
* Materials 2016, 9, 613 * 10 of 23
→ = = 4 cos + sin +

Beam CC` is fixed and therefore imposes no forces to point C. Force equilibrium at point C in the and directions gives (Figure 6c)

, = 0 → − cos sin +
12
cos sin +
4 = 0
→ = = 4 cos sin −
(19)
, = 0 → cos +
12
sin + _{2} = 0
→ = = −4 cos − sin
(20)

2.5.3. The Third DOF: = 1

This deformation type displaces vertex C upward by unity. Beam AB does not deform and, thus, does not impose any load to point B. Point A is not influenced by this deformation mode, thus

= = 0. Force equilibrium at point B in the direction gives (Figure 7a) , = 0 → 2 cos + 12 sin + 2 = 0 → = = −4 cos + sin (21)

Beam CC` (with length ℎ and cross-section area of /2) is stretched by 2 and therefore imposes the force AE /h to point C. Force equilibrium at point C in the X direction gives (Figure 7a)

, = 0 → − cos − 12

sin − _{ℎ} + _{4} = 0

→ = = cos + sin +

(22)

Similarly, force equilibrium at the same point in the direction gives (Figure 7a) , = 0 → cos sin − + 12 + 4 = 0 → = = cos sin − (23)

**Figure 7. Free-body diagrams of strut BC in deformations (a) ** **= 1; and (b) ** = 1.

**Materials 2016, 9, 613** 11 of 23

2.5.4. The Fourth DOF: q4“1

This deformation type displaces vertex C towards the left by unity. Similar to the case q3 “1, we have Q1“k14“0. Force equilibrium at point B and in the X2direction gives (Figure7b)

ÿ
fX2, B“0 Ñ ´2AEs
l *cosθsinθ `*
24EsI
l3 *cosθsinθ `*
Q2
2 “0
Ñ Q2“k24 “ˆ 4AEs
l ´
48EsI
l3
˙
*cosθsinθ*
(24)

Beam CC8simply displaces without any deformation, and therefore does not impose any load to point C. Force equilibrium in the X1direction at point C gives (Figure7b)

ÿ
fX2, C“0 Ñ ´AEs
l sin
2
*θ ´*12EsI
l3 cos
2
*θ `*Q4
4 “0
Ñ Q4“k44“
4AEs
l sin
2
*θ `*48EsI
l3 cos
2
*θ*
(25)

Similarly, force equilibrium at the same point in the X2direction gives (Figure7b)
ÿ
fX1, C“*0 Ñ cosθsinθ*
ˆ AEs
l ´
12EsI
l3
˙
`Q3
4 “0
Ñ Q3“k34 “*cosθsinθ*ˆ 48EsI
l3 ´
4AEs
l
˙ (26)

2.5.5. The Stiffness Matrix

Using the obtained stiffness matrix elements, the force-displacement relationship based on Euler-Bernoulli beam theory in the matrix form is

# Q1 Q2 Q3 Q4 + “ » — – 4AEs h ´ 4AEsh 0 0

´ 4AEs_{h} 4AEs_{l} *cos2 θ ` 48Es I*

l3 *sin2 θ ` 4AEs*h ´ 4AEsl *cos2 θ ´ 48Es I*l3 *sin2 θ*

ˆ 4AEs

l ´ 48Es Il3

˙
*cosθsinθ*

0 ´ 4AEs_{l} *cos2 θ ´ 48Es I*

l3 *sin2 θ*

48Es I

l3 *sin2 θ ` 4AEs*l *cos2 θ ` 4AEs*h

ˆ

´ 4AEs_{l} ` 48Es I

l3 ˙

*cosθsinθ*

0 4AEs_{l} *cosθsinθ ´ 48Es I*

l3 *sinθcosθ*
ˆ
48Es I
l3 ´ 4AEsl
˙
*cosθsinθ* 48Es I

l3 *cos2 θ ` 4AEs*l *sin2 θ*

fi ffi fl # q1 q2 q3 q4 + (27)

Comparison of Equations (10) and (16) shows that the matrix-form force-displacement relationship for the Timoshenko beam theory can be obtained by replacing 12EsI

l3 in Equation (27) by _{l3} 1
12Es I`*2κ AGs*l
which yields
$
’
’
’
&
’
’
’
%
Q1
Q2
Q3
Q4
,
/
/
/
.
/
/
/
-“
»
—
—
—
—
—
—
—
—
—
–
4AEs
h ´4AEsh 0 0

´4AEs_{h} 4AEs_{l} cos2* _{θ `}* 4
l3
12Es I`

*2κ AGs*l sin2

*4AEs h ´4AEsl cos2*

_{θ `}*θ ´*l3 4 12Es I`

*2κ AGs*l sin2

*ˆ 4AEs l ´ l3 4 12Es I`*

_{θ}*2κ AGs*l ˙

*cosθsinθ*0 ´4AEs

_{l}cos2

*4 l3 12Es I`*

_{θ ´}*2κ AGs*l sin2

*θ*

_{l3}4 12Es I`

*2κ AGs*l

sin2*θ `*4AEs_{l} cos2* _{θ `}*4AEs
h
ˆ
´4AEs

_{l}`

_{l3}4 12Es I`

*2κ AGs*l ˙

*cosθsinθ*0 4AEs l

*cosθsinθ ´*l3 4 12Es I`

*2κ AGs*l

*sinθcosθ*ˆ 4 l3 12Es I`

*2κ AGs*l ´4AEs

_{l}˙

*cosθsinθ*4 l3 12Es I`

*2κ AGs*l cos2

*4AEs l sin2*

_{θ `}*θ*fi ffi ffi ffi ffi ffi ffi ffi ffi ffi fl $ ’ ’ ’ & ’ ’ ’ % q1 q2 q3 q4 , / / / . / / / -(28)

Since point B is an internal vertex, no external force is applied to it. The external force applied
to point C in the X2direction is zero, thus Q2“Q3 “0. If the stress acting on the structure in the
X1*direction is denoted by σ*x, using the geometrical relations, the force acting on point C in the X1
*direction can be obtained as 2 ph ` lcosθq σ*1b, where b is the thickness of the honeycomb structure in

**Materials 2016, 9, 613** 12 of 23

its out of plane direction. Similarly, the force acting on point A in the X2direction is calculated as
*2lsinθ σ*2*b, where σ*2is the stress acting on the structure in the X2direction. The force vector is therefore

$
’
’
’
&
’
’
’
%
Q1
Q2
Q3
Q4
,
/
/
/
.
/
/
/
-“
$
’
’
’
&
’
’
’
%
*2 r2lsinθσ*2bs
0
0
*4 r2 ph ` lcosθq σ*1bs
,
/
/
/
.
/
/
/
-“
$
’
’
’
&
’
’
’
%
*4lsinθσ*2b
0
0
*8 ph ` lcosθq σ*1b
,
/
/
/
.
/
/
/
-(29)

2.6. The Obtained Elastic Properties

For any deformation, the unknown displacements can be simply obtained by inverting the stiffness
matrix given in Equations (27) or (28) and multiplying it by the force vector given in Equation (29).
Using the obtained unknowns, it is possible to calculate the elastic modulus, Poisson’s ratio, and yield
stress of the honeycomb structure as functions of the geometrical and material properties Es*, σ*ys*, ν*s.
2.6.1. Elastic Modulus

The elastic modulus in each direction is found by dividing the applied stress in that direction by
the resulting strain in that direction, i.e., E1*“ σ*1*{ε*1*“ σ*1plsinθq {q4and E2*“ σ*2*{ε*2*“ σ*2ph ` lcosθq {q1.
Using the Euler-Bernoulli stiffness matrix, the relative elastic modulus in the X1direction is obtained as

ˆ E
Es
˙
1
“ t
3
l3
*l sinθ*

*h pcosθ ` 1q*´sin2*θ*`t_{l}˘2 ` cos2* _{θ}*¯ (30)
and using the Timoshenko stiffness matrix, the relative elastic modulus in the X1 direction is
obtained as
ˆ E
Es
˙
1
“ t
3
l3

*l sinθ*

*h pcosθ ` 1q*´ cos2

_{θ `}_{0.2}`

_{t}l ˘2 cos2

*`*

_{θ `}_{t}l ˘2 `

*1.1 ν*s `

_{t}l ˘2 cos2

*¯ (31) The relative elastic modulus in the X2direction for the Euler-Bernoulli beam theory is*

_{θ}ˆ E
Es
˙
2
“ t
3
l3
h
l ` *cosθ*

*sinθ*´2h_{l} `t_{l}˘2 ` `t_{l}˘2 cos2* _{θ ` sin}*2

*θ*

¯ (32)

and for the Timoshenko beam theory is
ˆ E
Es
˙
2
“ t
3
l3
h
l `*cosθ*
*sinθ*´2h_{l} `t_{l}˘2``t_{l}˘2 `sin2*θ*
¯
`sin3*θ*
´
0.2`t_{l}˘2`1.1`t_{l}˘2 *ν*s
¯ (33)
2.6.2. Poisson’s Ratio

The Poisson’s ratio can be obtained by dividing the two strains in the X1*directions. For ν*12, we
*have ν*12 “ *ε2 _{ε1}* “ qq

_{4}1 ph`lcosθq

*l sinθ*

*for σ*1 ‰

*0 and σ*2 “0. Using the Euler-Bernoulli force-displacement

*relationship (i.e., Equation (27)), the Poisson’s ratio ν*12is found as

*ν*12“
lsin2*θcosθ*`l2´t2˘
´
t2_{sin}2
*θ ` l*2cos2*θ*
¯
ph ` lcosθq
(34)

and for Timoshenko beam theory, it is

*ν*12“

lsin2*θcosθ* `l2` 0.2 t2` 1.1 t2*ν*s
˘

`l2_{cos}2_{θ `}_{0.2 t}2_{cos}2* _{θ ` t}*2

_{`}

_{1.1 t}2

_{cos}2

_{θν}_{s}˘

**Materials 2016, 9, 613** 13 of 23

*For ν*21*, we have ν*21“ *ε1 _{ε2}* “ qq4

_{1}

ph`lcosθq

*l sinθ* *for σ*2‰*0 and σ*1“0, which for the Euler-Bernoulli beam
theory gives

*ν*21 “

*cosθsinθ*`l2´ t2˘ph ` l cosθq

*sinθ*`2ht2_{`} _{t}2_{lcos}2* _{θ ` l}*3

_{sin}2

*˘ (36)*

_{θ}and for the Timoshenko beam theory, it is

*ν*12“

*cosθ sinθ ph ` lcosθq* `l2 ` 0.2 t2 ` 1.1 t2*ν*s
˘

*sinθ* `l3_{sin}2

*θ `*2 t2h ` t2l ` 0.2 t2l sin2*θ `*1.1 t2*l ν*ssin2*θ*˘

(37)

2.6.3. Yield Stress

In the FE simulations, it was seen that that the end points of the inclined edges are the location
with maximum stress for all cases of axial loading in the X1direction, axial loading in the X2direction,
and bi-axial loading. In a general deformation of beam BC, in which point B is dislocated by q2
in the X2direction and point C is dislocated by q4and q3respectively in the X1and X2directions,
by assuming that beam BC is clamped at one of its ends B or C, increase in the length of the beam
BC is q4*sinθ ` pq*2´q3q*cosθ. Similarly, the relative lateral displacement of the free end of beam BC*
is pq2´q3q*sinθ ´ q*4*cosθ. These displacements cause axial load (Figure*5b) and bending moments
(Figure5a) in the beam

P “ AEs

l pq4*sinθ ` pq*2´q3q*cosθq*
M “ 6EsI

l2 ppq2´q3q*sinθ ´ q*4*cosθq*

(38)

which impose the axial and flexural stresses of
*σ*axial“
Es
l pq4*sinθ ` pq*2´q3q*cosθq*
*σ*_{f lexure}“ 3Est
l2 ppq2´q3q*sinθ ´ q*4*cosθq*
(39)

By adding the axial and flexural stresses given in the above equation, the maximum stress in the honeycomb unit cell can be found. The yield stress of the structure is then given by

*σ*y“
*σ*ys*σ*i

*σ*max (40)

*where σ*ys*is the yield stress of the bulk material, σ*i*is the applied stress in direction i, and σ*max is the
*resulting maximum stress σ*max *“ σ*axial*` σ*f lexure. The relative yield stress in the X1direction for the
Euler-Bernoulli beam theory is found as

ˆ
*σ*y
*σ*ys
˙
1
“ 1
*h p1 ` cosθq*
ˆ
t2
*t sinθ ` 3l cosθ*
˙
(41)
The analytical relationship for the yield stress based on the Timoshenko beam theory was lengthy
and, had limited influence on the yield stress. We therefore do not present the analytical relationship
for the yield stress in the X1direction based on the Timoshenko beam theory. The relative yield stress
in the X2direction was found as

ˆ
*σ*y
*σ*ys
˙
2
“ 1
*l sinθ*
ˆ
t2
*3l sinθ ´ t cosθ*
˙
(42)

**Materials 2016, 9, 613** 14 of 23

for the Euler-Bernoulli beam theory and
ˆ
*σ*y
*σ*ys
˙
2
“ 1
*l sinθ*
˜
t2

*3l sinθ ´ tcosθ ` 3*t_{l}2p1.2 ` 1.1νsq*sinθ*
¸

(43) for the Timoshenko beam theory.

2.7. Computational Modelling

In this study, FE simulations were used as a validation tool for the analytical relationships
derived above. The planar deformation of the honeycomb structures suggests using beam elements
for representing the cell edges. All the links in the hexagonal honeycomb structure were represented
mechanically by beams that were rigidly connected at the vertices. The edges were discretized using
the standard Timoshenko beam elements that uses linear interpolation approximation and allows for
transverse shear deformation. Considering transverse shear deformation becomes more important in
thick beams (such as the ones constructing a high density honeycomb) compared to slender beams.
Since in this study, the mechanical properties of the honeycomb are obtained in elastic regime, and
since the results are reported in normalized values, the type of material for the FE modelling does not
affect the results (i.e., the normalized values of mechanical properties). The material considered for the
numerical analysis was steel and its mechanical behavior was assumed to be linear elastic, with the
elastic modulus Es “ *200 GPa and the Poisson’s ratio ν*s “ 0.3.

The static nonlinear implicit solver of ANSYS FE code was used for solving the problem. The geometry of the FE model (Figure8) was identical to the geometry of the unit cell used for the analytical derivations (Figure2). All the vertices were constrained in the X3direction (perpendicular to the page). The vertices A, B, A8, and B8 connected to the two vertical beams AB and A8B8 were constrained in the X1direction (see Figure2). In order to avoid singularity of the pivot terms in the ANSYS solver caused by rigid body movements, the degrees of freedom of one of the vertices must be completely constrained in the space. Since this structure has no central vertex, the bottom point A8 was fixed in space.

* Materials 2016, 9, 613 * 14 of 23

mechanically by beams that were rigidly connected at the vertices. The edges were discretized using the standard Timoshenko beam elements that uses linear interpolation approximation and allows for transverse shear deformation. Considering transverse shear deformation becomes more important in thick beams (such as the ones constructing a high density honeycomb) compared to slender beams. Since in this study, the mechanical properties of the honeycomb are obtained in elastic regime, and since the results are reported in normalized values, the type of material for the FE modelling does not affect the results (i.e., the normalized values of mechanical properties). The material considered for the numerical analysis was steel and its mechanical behavior was assumed to be linear elastic, with the elastic modulus = 200 and the Poisson’s ratio = 0.3.

The static nonlinear implicit solver of ANSYS FE code was used for solving the problem. The geometry of the FE model (Figure 8) was identical to the geometry of the unit cell used for the analytical derivations (Figure 2). All the vertices were constrained in the direction (perpendicular to the page). The vertices A, B, A`, and B` connected to the two vertical beams AB and A`B` were constrained in the direction (see Figure 2). In order to avoid singularity of the pivot terms in the ANSYS solver caused by rigid body movements, the degrees of freedom of one of the vertices must be completely constrained in the space. Since this structure has no central vertex, the bottom point A` was fixed in space.

**(a) (b)**

**Figure 8. (a) The geometry, loads, and boundary conditions used in the 2D hexagonal honeycomb **

**finite element (FE) model; and (b) its deformed shape, for ** 0 and = 0.

The elastic modulus of the structure in each direction was calculated by applying a uniaxial stress and measuring the resulting strain in the same direction and then dividing both values, i.e., = . The Poisson’s ratios were determined by dividing the negative value of the lateral strain by the axial strain. The yield stress was found by finding the maximum stress, , in the FE model and then substituting it in Equation (40).

**3. Results **

All the samples showed 45° failure bands during their post yielding behavior (Figure 9). Since the experimental data provided by Gibson and Ashby [10,27] are only presented for very small relative densities ( 0.02) and the experimental results obtained in this paper cover relatively large relative densities (0.2 0.55), the diagram of each mechanical behavior is plotted in two ranges of relative densities: one from 0 to 0.02, and the other from 0 to 0.5. At very small relative densities, the elastic modulus obtained from the derived analytical formulas (based on both Timoshenko and Euler-Bernoulli beam theories), the analytical formulas presented by Gibson and Ashby [10,27] and Masters [22], the FE model, and Gibson and Ashby [10,27] experimental observations all coincide well with each other (Figures 10a and 11a), but they start to deviate from each other as the relative density of the structure increases. For a relative density of 0.5, the elastic modulus predicted by the

**Figure 8.(a) The geometry, loads, and boundary conditions used in the 2D hexagonal honeycomb**

* finite element (FE) model; and (b) its deformed shape, for σ*1‰

*0 and σ*2“0.

The elastic modulus of the structure in each direction was calculated by applying a uniaxial
*stress σ*i*and measuring the resulting strain in the same direction ε*iand then dividing both values, i.e.,
Ei“ *σ _{εi}*i. The Poisson’s ratios were determined by dividing the negative value of the lateral strain by

**Materials 2016, 9, 613** 15 of 23

*the axial strain. The yield stress was found by finding the maximum stress, σ*max, in the FE model and
then substituting it in Equation (40).

**3. Results**

All the samples showed 45˝_{failure bands during their post yielding behavior (Figure}_{9}_{). Since the}
experimental data provided by Gibson and Ashby [10,27] are only presented for very small relative
*densities (µ ă 0.02) and the experimental results obtained in this paper cover relatively large relative*
*densities (0.2 ă µ ă 0.55), the diagram of each mechanical behavior is plotted in two ranges of*
relative densities: one from 0 to 0.02, and the other from 0 to 0.5. At very small relative densities,
the elastic modulus obtained from the derived analytical formulas (based on both Timoshenko and
Euler-Bernoulli beam theories), the analytical formulas presented by Gibson and Ashby [10,27] and
Masters [22], the FE model, and Gibson and Ashby [10,27] experimental observations all coincide
well with each other (Figures10a and11a), but they start to deviate from each other as the relative
density of the structure increases. For a relative density of 0.5, the elastic modulus predicted by the
Gibson and Ashby formula is almost twice that obtained from the analytical Timoshenko formula
(i.e., Equations (31) and (33)) and the FE model (Figures10b and11b).

* Materials 2016, 9, 613 * 15 of 23

Gibson and Ashby formula is almost twice that obtained from the analytical Timoshenko formula (i.e., Equations (31) and (33)) and the FE model (Figures 10b and 11b).

**Figure 9. The 45° failure pattern in the honeycombs. **

**(a)**
0 0.005 0.01 0.015 0.02
0
0.5
1
1.5x 10
−5
**Relative density**

**Normalized elastic modulus (E/E**

**s**
**) in X**
**1**
** direction**
**Theory (Euler−Bernoulli)**
**Theory (Timoshenko)**
**Theory (Gibson and Ashby, 1997)**
**Theory (Masters and Evans, 1996)**
**Finite element**

**Experiment (Gibson and Ashby, 1997)**

**Materials 2016, 9, 613** 16 of 23

* Materials 2016, 9, 613 * 15 of 23

Gibson and Ashby formula is almost twice that obtained from the analytical Timoshenko formula (i.e., Equations (31) and (33)) and the FE model (Figures 10b and 11b).

**Figure 9. The 45° failure pattern in the honeycombs. **

**(a)**
0 0.005 0.01 0.015 0.02
0
0.5
1
1.5x 10
−5
**Relative density**

**Normalized elastic modulus (E/E**

**s**
**) in X**
**1**
** direction**
**Theory (Euler−Bernoulli)**
**Theory (Timoshenko)**
**Theory (Gibson and Ashby, 1997)**
**Theory (Masters and Evans, 1996)**
**Finite element**

**Experiment (Gibson and Ashby, 1997)**

* Materials 2016, 9, 613 * 16 of 23

**(b)**

**Figure 10. Variation of relative elastic modulus in ** direction ( / ) vs. relative density ( / ) for

**analytical, experimental, and numerical results. (a) For small relative density range; and (b) for the **
complete range of relative density.

**(a)**

**(b)**

**Figure 11. Variation of relative elastic modulus in ** direction ( / ) vs. relative density ( / ) for

**analytical, experimental, and numerical results. (a) For small relative density range; and (b) for the **
complete range of relative density.

0 0.1 0.2 0.3 0.4 0.5 0.6
0
0.05
0.1
0.15
0.2
0.25
0.3
0.35
**Relative density**

**Normalized elastic modulus (E/E**

**s**
**) in X**
**1**
** direction**
**Theory (Euler−Bernoulli)**
**Theory (Timoshenko)**
**Theory (Gibson and Ashby, 1997)**
**Theory (Masters and Evans, 1996)**
**Finite element**

**Experiment (Current study)**

0 0.005 0.01 0.015 0.02
0
0.5
1
1.5x 10
−5
**Relative density**

**Normalized elastic modulus (E/E**

**s**
**) in X**
**2**
** direction**
**Theory (Euler−Bernoulli)**
**Theory (Timoshenko)**
**Theory (Gibson and Ashby, 1997)**
**Theory (Masters and Evans, 1996)**
**Finite element**

**Experiment (Gibson and Ashby, 1997)**

0 0.1 0.2 0.3 0.4 0.5 0.6
0
0.05
0.1
0.15
0.2
0.25
0.3
0.35
**Relative density**

**Normalized elastic modulus (E/E**

**s**
**) in X**
**2**
** direction**
**Theory (Euler−Bernoulli)**
**Theory (Timoshenko)**
**Theory (Gibson and Ashby, 1997)**
**Theory (Masters and Evans, 1996)**
**Finite element**

**Experiment (Current study)**

**Figure 10.**Variation of relative elastic modulus in X1direction (E1{Es*) vs. relative density (ρ{ρ*s) for

**analytical, experimental, and numerical results. (a) For small relative density range; and (b) for the**
complete range of relative density.

For large relative densities, the analytical elastic modulus formulas presented by Gibson and Ashby deviate significantly from the other results, i.e., the Euler-Bernoulli beam theory (obtained in this study and obtained by Masters and Evans [22]), the Timoshenko beam theory, the numerical results, and the experimental data of the tests carried out in this study (Figures10b and11b). The elastic modulus formulas presented by Masters and Evans [22] and the Euler-Bernoulli-based formulas obtained in this study rely on each other for all the values of relative density. Moreover, the elastic modulus obtained based on the Timoshenko beam theory is smaller than that based on the Euler-Bernoulli beam theory and is generally in better agreement with numerical results (Figures10b and11b). Compared to Gibson and Ashby analytical formulas and the derived Euler-Bernoulli theory, the Timoshenko analytical elastic modulus presented in this study corresponds much better with both experimental and numerical results.

**Materials 2016, 9, 613** 17 of 23

* Materials 2016, 9, 613 * 16 of 23

**(b)**

**Figure 10. Variation of relative elastic modulus in ** direction ( / ) vs. relative density ( / ) for

**(a)**

**(b)**

**Figure 11. Variation of relative elastic modulus in ** direction ( / ) vs. relative density ( / ) for

0 0.1 0.2 0.3 0.4 0.5 0.6
0
0.05
0.1
0.15
0.2
0.25
0.3
0.35
**Relative density**

**Normalized elastic modulus (E/E**

**s**
**) in X**
**1**
** direction**
**Theory (Euler−Bernoulli)**
**Theory (Timoshenko)**
**Theory (Gibson and Ashby, 1997)**
**Theory (Masters and Evans, 1996)**
**Finite element**

**Experiment (Current study)**

0 0.005 0.01 0.015 0.02
0
0.5
1
1.5x 10
−5
**Relative density**

**Normalized elastic modulus (E/E**

**s**
**) in X**
**2**
** direction**
**Theory (Euler−Bernoulli)**
**Theory (Timoshenko)**
**Theory (Gibson and Ashby, 1997)**
**Theory (Masters and Evans, 1996)**
**Finite element**

**Experiment (Gibson and Ashby, 1997)**

0 0.1 0.2 0.3 0.4 0.5 0.6
0
0.05
0.1
0.15
0.2
0.25
0.3
0.35
**Relative density**

**Normalized elastic modulus (E/E**

**s**
**) in X**
**2**
** direction**
**Theory (Euler−Bernoulli)**
**Theory (Timoshenko)**
**Theory (Gibson and Ashby, 1997)**
**Theory (Masters and Evans, 1996)**
**Finite element**

**Experiment (Current study)**

**Figure 11.**Variation of relative elastic modulus in X2direction (E2{Es*) vs. relative density (ρ{ρ*s) for

*The formulas presented by Gibson and Ashby predict a constant Poisson’s ratio (i.e., ν “ 1) for*
all values of relative density. Both the analytical formulas derived in this paper and our FE results,
coincide with the Gibson and Ashby result at very small relative densities, but start to decrease as the
relative density increases (Figure12). The FE results almost coincide with the analytical results obtained
using the Timoshenko beam theory. Moreover, the Poisson’s ratio formulas presented by Masters [22]
and the Euler-Bernoulli-based formulas derived here lie on top of each other. The Poisson’s ratio
value is identical in the X1and X2*directions for both numerical and analytical results (ν*12 *“ ν*21).
*At µ “ 0.5, the predicted Poisson’s ratios obtained from all the methods implemented in this study are*
all between 0.5 and 0.6, which is in contrast with the prediction of Gibson and Ashby theory which is 1.
The experimental results obtained from a number of tests carried out by Gibson and Ashby [10,27]
also show much smaller Poisson’s ratio than their theoretical predictions.

**Materials 2016, 9, 613** 18 of 23

* Materials 2016, 9, 613 * 17 of 23

For large relative densities, the analytical elastic modulus formulas presented by Gibson and Ashby deviate significantly from the other results, i.e., the Euler-Bernoulli beam theory (obtained in this study and obtained by Masters and Evans [22]), the Timoshenko beam theory, the numerical results, and the experimental data of the tests carried out in this study (Figures 10b and 11b). The elastic modulus formulas presented by Masters and Evans [22] and the Euler-Bernoulli-based formulas obtained in this study rely on each other for all the values of relative density. Moreover, the elastic modulus obtained based on the Timoshenko beam theory is smaller than that based on the Euler-Bernoulli beam theory and is generally in better agreement with numerical results (Figures 10b and 11b). Compared to Gibson and Ashby analytical formulas and the derived Euler-Bernoulli theory, the Timoshenko analytical elastic modulus presented in this study corresponds much better with both experimental and numerical results.

The formulas presented by Gibson and Ashby predict a constant Poisson’s ratio (i.e., = 1) for all values of relative density. Both the analytical formulas derived in this paper and our FE results, coincide with the Gibson and Ashby result at very small relative densities, but start to decrease as the relative density increases (Figure 12). The FE results almost coincide with the analytical results obtained using the Timoshenko beam theory. Moreover, the Poisson’s ratio formulas presented by Masters [22] and the Euler-Bernoulli-based formulas derived here lie on top of each other. The

Poisson’s ratio value is identical in the and directions for both numerical and analytical

results ( = ). At = 0.5 , the predicted Poisson’s ratios obtained from all the methods

implemented in this study are all between 0.5 and 0.6, which is in contrast with the prediction of Gibson and Ashby theory which is 1. The experimental results obtained from a number of tests carried out by Gibson and Ashby [10,27] also show much smaller Poisson’s ratio than their theoretical predictions.

**Figure 12. Comparison of analytical and numerical values of Poisson’s ratio for different relative **

densities.

Unlike the elastic modulus and Poisson’s ratio for which all the numerical and analytical methods gave very close results at small relative densities, the analytical formulas given by Gibson and Ashby predict different yield stresses even at small relative densities (Figure 13). The analytical formulas obtained in this study, the FE model, and Gibson and Ashby’s experimental data are in good agreement for small relative densities, but the analytical formulas presented by Gibson and Ashby are somewhat different from all other results (Figures 13a and 14a). For example, for a small relative density of 0.02, the yield stress predicted by Gibson and Ashby formulas is about 30% higher than those predicted by other techniques. This deviation continues to increase for larger relative densities, especially in the X direction (Figure 14b). At the relative density of 0.5, the yield stress predicted analytically by the relationships presented in the Gibson and Ashby study is at least twice that given by other techniques. The analytical relationships derived using both Euler-Bernoulli

0 0.1 0.2 0.3 0.4 0.5
0
0.2
0.4
0.6
0.8
1
**Relative density**
**Poisson‘s ratio**

** _{12} and **

_{21}(Euler−Bernoulli theory)** _{12} and **

_{21}(Timoshenko theory)** _{12} and **

_{21}(Gibson and Ashby theory, 1997)** _{12} and **

_{21}(Masters and Evans theory, 1996)_{12} (Finite element)

_{21} (Finite element)

**Figure 12.** Comparison of analytical and numerical values of Poisson’s ratio for different

relative densities.

* Materials 2016, 9, 613 * 18 of 23

and Timoshenko theories almost coincide for relative densities smaller than 0.15 (Figures 13 and 14). For all relative densities, the yield stress formula based on the Timoshenko beam theory correlates well with the experimental tests carried out in this study, Gibson and Ashby’s experimental results, and the FE results (Figure 13).

**(a)**

**(b)**

**Figure 13. Variation of relative yield stress in ** direction / vs. relative density ( / ) for

It is noteworthy to mention that the analytical relationships derived for the Poisson’s ratio and elastic modulus are identical in both major directions and (see Figure 12 and compare Figure 10 and Figure 11). Therefore, the reciprocal relationship = is also valid for the honeycomb. However, the structure shows a higher yield stress in the X direction. For example at

= 0.5, the yield stress in the direction is 18.5% higher than that in the direction. This large difference in the yield stress in both major directions disappears for small values of relative density

0 0.005 0.01 0.015 0.02
0
1
2
x 10−4
**Relative density**

**Normalized yield stress (**

**y**
**/**
**ys**
**)**
**Theory (Euler−Bernoulli)**
**Theory (Timoshenko)**

**Theory (Gibson and Ashby, 1997)**
**Finite element**

**Experiment (Gibson and Ashby, 1997)**

0 0.1 0.2 0.3 0.4 0.5 0.6
0
0.02
0.04
0.06
0.08
0.1
0.12
0.14
0.16
0.18
0.2
**Relative density**

**Normalized yield stress (**

**y**
**/**
**ys**
**)**
**Theory (Euler−Bernoulli)**
**Theory (Timoshenko)**

**Theory (Gibson and Ashby, 1997)**
**Finite element**

**Experiment (Current study)**

**Figure 13.** Variation of relative yield stress in X1direction

`

*σ*y*{σ*ys˘_{1} *vs. relative density (ρ{ρ*s) for